1 Academia Journal of Food Research 4(1): , July 2016 DOI: /ajfr ISSN: Academia Publishing Research Paper Physico-mechanical and antioxidant properties of carboxymethylcellulose and alginate dispersions and essential oil based films for use as food packaging materials Accepted 19 th May, 2016 ABSTRACT Mohammadreza Raisi-Nafchi 1, Gholamreza Kavoosi 1 * and Seyed Mehdi Nasiri 2 1 Institute of Biotechnology, Shiraz University, Shiraz, , Iran. 2 Department of Biosystem Engineering, Shiraz University, Shiraz, , Iran. *Corresponding author Tel: Fax; Oxidative corrosion presumably has a great contribution in reducing nutritional and sensory quality of food products by deteriorating vitamins and unsaturated fatty acids and also affecting the shelf-life of foodstuff. In the present research, physical and antioxidant properties of 3% w/v of carboxy methyl cellulose (CMC) and alginate (ALG) filmogenic dispersions (FD) and film and their blends CMC/ALG enriched with 8% w/w of Zataria multiflora essential oil (ZO) as a food packaging material were examined. To achieve this goal, impacts of polymer blending as well as, ZO incorporation on the properties of FD and film were evaluated. According to the results, by adding polymer blends and ZO, ph, conductivity, ζ-potential, particle size, viscosity, light barrier and antioxidant activity of FD changed significantly for per type of blends and ZO content. Variations in the properties of filmogenic dispersions denoted an interaction between CMC and alginate molecules ZO. Mechanical and water barrier properties of the films might be affected by such interaction. Polymer blend and ZO caused a significant change in films mechanical and water binding properties. As atomic force microscope analyses showed, ZO induced changes in the films surface topography through increasing surface roughness. The antioxidant filmogenic dispersions dealt with in this study is promising to be used as a natural antioxidant additive and a substitution for synthetic antioxidants. It also reduces oxidative deterioration of foodstuff and improves the shelf-life of food. Key words: CMC, ALG, dispersion, zataria oil, rheology, antioxidant. INTRODUCTION Biodegradable film production based on polysaccharide biopolymer is characterized with strong anti-oxidant and antibacterial properties and serves as a strategic choice concerning mega trends in global health. Some of these biopolymers such as, carboxy methyl cellulose (CMC) and alginate (ALG) are proven to have high potential in food and pharmaceutical applications as they have strong gelforming properties. As a renewable material, CMC has desirable characteristics such as substantial mechanical properties, water absorbency, biodegradability and biocompatibility. It has wide variety of applications in biomedical fields including a biomaterial for artificial skin, artificial blood vessels, vascular grafts and a scaffold for tissue engineering and wound dressing (Shah et al., 2013). Food ingredients for thickening, gelling, stabilizing, water binding and packaging materials are found to be multifunctional properties of CMC-based materials (Shi et al., 2013). Alginate is an anionic polymer naturally derived from brown seaweed and has been extensively applied in food and biomedical industry oweing to its biocompatibility,
2 Academia Journal of Food Research; Raisi-Nafchi et al. 002 low toxicity and excellent gel formation capacity properties (Pawar and Edgar, 2012). Alginate-based materials are found to be characterized by multi-functional properties; alginate hydrogels, for instance, have been widely applied in wound healing, drug delivery and tissue engineering mostly because of their structural affinity to extracellular matrices of living tissues (Lee and Mooney, 2012). On the other side, CMC and ALG based materials do not have inherent anti-oxidant properties. In spite of great applications of synthetic anti-oxidants in various medical and food fields, plant extracts and essential oils as natural sources of anti-oxidant compounds in the formulation of CMC and ALG based materials have been receiving great deals of attentions (Gomez-Estaca et al., 2014). Sanchez- Gonzalez et al. (2009) in their study shed lights on transparency and mechanical properties of hydroxypropylmethylcellulose incorporated with tea tree essential oil. At the same time, anti-microbial and antioxidant activities in CMC edible films containing rosemary extract was reported by Liu et al. (2012). Ramirez et al. (2012) studied wettability and water vapor permeability in murta leaves extract based- CMC films. In addition, physical and antioxidant activities in methylcellulosebased films containing resveratrol was found by Pastor et al. (2013). Finally, the remarkable anti-microbial and antifungal properties of films made of lavender, tea tree, peppermint, eucalyptus, cinnamon and lemongrass oils dispersed in sodium alginate were found by Liakos et al. (2014). Nonetheless, it is noteworthy that to the best of our knowledge there are paucity of studies conducted on the rheological properties of filmogenic dispersion (FD) incorporated with essential oil. Zataria multiflora, a thyme-like plant belonging to the Lamiaceae family, is another promising plant used to activate CMC and ALG based materials. Foregoing species has several functional properties and is renowned for its anti-septic, vermifuge, anti-helminthes, carminative, diaphoretic, diuretic, anesthetic, anti-spasmodic, antidiarrheal, analgesic and anti-tussive activities (Sajed et al., 2013). As a good source of phenolic monoterpenes (thymol and carvacrol) Z. multiflora essential oil (ZO) has strong anti-oxidant activity and good anti-inflammatory properties (Kavoosi and Rabiei, 2015). As earlier illustrated, there is a paucity of literatures on the physical properties and anti-oxidant activity of CMC and ALG FD and their ZO-based composites. Here, CMC and ALG FD and their composites CMC/ALG were prepared and incorporated with ZO. Then, we shed lights on properties, including density, ph, conductivity, ζ-potential, particle size, viscosity, light barrier and antioxidant properties of the FD. A comparison was carried out on films mechanical properties and their composites, casted from FD, such as tensile strength, elastic modulus and elongation at break. The research was conducted in two steps: we explained effects of polymer blending on the properties of filmogenic dispersions and film followed by effects of ZO on the properties of filmogenic dispersions and film. MATERIALS AND METHODS Materials Sodium alginate (low viscosity) and CMC (low viscosity) were purchased from Sigma-Aldrich chemical Co. (Saito Louis, Mo, USA). All other chemicals, including 1, 1- diphenyl-2-picryl-hudrazyl radical (DPPH ), 2, 2-azino-bis (3-ethylbenzthiazoline-6-sulfonic acid) and radical (ABTS ) were of analytical grade and purchased from Sigma chemical Co. (Saito Louis Mo, USA). To extract ZO, the air-dried leaves (100 g) were dissolved in 1000 ml distilled water. The acquired mixture was exposed to hydro-distillation for 4 h using an all glass Clevenger type apparatus. ZO was dehydrated over anhydrous sodium sulphate and stored at 4 to 6 C. To calculate ZO, density digital balance was considered and the average found to be 996 mg/ml. Thus, each µl of ZO approximately equals to 1 mg. ZO were dissolved in one volume of tween 20 thus, the final concentration of emulsified ZO was consiedered as 500 mg/ml. Preparation and characterization of FD In order to prepare CMC, ALG and CMC/ALG (1:1) dispersion one gram of each polymer was dissolved in 80 ml of distilled water under continuous stirring at 40 C until a homogenous solution was obtained. The homogenous PVP solution was sonicated using an ultrasonic (Bandlin, Germany) at 140 W for 5 min at the temperature 30 C. To prepare CMC/ZO, ALG/ZO and CMC/ALG/ZO dispersions, ZO (100 mg/g of polymer) was added to the dispersions and mixed under mechanical stirring at 800 RPM for 12 h at 40 C. As an emulsifier, glycerol (300 mg/g PVP) was added to all dispersions and mixed under mechanical stirring at 800 RPM at 40 C. At the end, distilled water was added until the final volume reached 100 ml under mechanical stirring at 800 RPM at 40 C. The final dispersions were stored at 4 C for further experiments. Before physical tests, the dispersions were equilibrated at room temperature (25 to 27 C) for 3 h to reach a constant temperature. The dispersions were stable for at least 100 days as checked by visual observation through testing phase separation (Goh et al., 2012; Sanchez-Gonzalez et al., 2011). Density and ph of FD The FD density was analyzed through weighing 1 ml of the FD using digital balance (Acculab, Sartorius group, Germany) and expressed in mg/ml. Mettler-Toledo instrument (Cleantech, Schaffhausen, Switzerland) was
3 Academia Journal of Food Research; Raisi-Nafchi et al. 003 used to measure the ph and conductivity of the FD. Zeta-potential of particle The dispersions were diluted to a final concentration of 50 µg/ml by deionized water. The electrophoretic mobility of particles in the dispersion was determined by Phase Analysis Light Scattering (PALS) technique using a Brookhaven instruments corporation 90 Plus zeta-sizer (New York, 11742, USA). The Bi-PALS zeta potential analyzer software provided an average of electrophoretic mobility and a measure of zeta-potential using smolouchewsky model (De Oliveira et al., 2014). Effective hydrodynamic diameter of particle The dispersions were diluted to a final concentration of 50 µg/ml of deionized water. The effective hydrodynamic diameter of particles was determined based on the principle of dynamic light scattering (DLS) using a Brookhaven instrument corporation 90 Plus particle size analyzer. The Bi-9000 particle sizing software provided an average effective hydrodynamic diameter of the particles (Sanchez-Gonzalez et al., 2009). Apparent viscosity The dispersions were decanted into a 200 ml glass cylinder (80 mm 70 mm) and left on an anti-vibration bench with a flat level for 10 min to equilibrate. The apparent viscosities (mpa.s) of the dispersions were quantified through the use of Brookfield viscometer (DV-II + PRO digital viscometer, Meddleboro, USA, spindle 2) at spindle rotational speed of 1, 2, 5 and 10 s -1. The software of Brookfield instrument directly provided the apparent viscosity of the dispersions (Fu et al., 2011). ABTS radical scavenging assay of FD Twenty microliters of each FD ( µg/ml) were added to 1 ml of diluted ABTS radical solution (7 mm ABTS and 2.54 mm potassium persulfate). Once mixed, the absorbance (A) was read at 734 nm using Unico 2100 spectrophotometer. ABTS scavenging percentage was estimated through the following formula given as: ABTS scavenging (%) = [(A ABTS - A test) / A ABTS ] 100. Where, A ABTS is the absorbance of ABTS solution and A test is the absorbance of ABTS solution in the presence of FD. The concentrations that could provide 50% ABTS scavenging (IC 50) were calculated by the graph plotted on the inhibition percentage versus different concentrations of the FD. ABTS scavenging power of FD was calculated employing the following formula: [1000/IC 50] 100 (Floegel et al., 2011). DPPH radical scavenging activity of FD Twenty microliters of each FD ( µg/ml) were added to 2 ml of 0.2 mm DPPH in 95% methanol. The mixture stored for 30 min at room temperature at night. Unico 2100 spectrophotometer was applied to assess reduction in each sample light absorbance (A) at 517 nm (Figure 1). DPPH scavenging activity was expressed as DPPH scavenging percentage using the formula: DPPH scavenging (%) = [(A DPPH - A test) / A DPPH ] 100. Where, A DPPH = absorbance of DPPH solution and A test = absorbance of DPPH solution in the presence of FD. The IC 50 was calculated from the graph plotting the DPPH scavenging percentage versus different FD concentrations. DPPH scavenging power of FD was calculated the given formula: [1000/IC 50] 100 (Floegel et al., 2011). Preparation and characterization of films The FD was poured into flat and leveled polystyrene petri dishes (Farazbin, Tehran, Iran) for film casting. Once set, the petri dishes were held overnight at 50 C in a vacuum oven (Fan Azma Gostar, Tehran, Iran) for 12 h to bring out a uniform thickness followed by cooled to ambient temperature before peeling them off the petri dishes (Sanchez-Gonzalez et al., 2009, 2011). The film samples were stored in plastic bags and held in desiccators at 60 ± 5% relative humidity over a saturated solution of Mg(NO 3) 2.6H 2O for further testing. Mechanical behavior of the films Tensile strength (TS), elongation at break (EB), and elastic modulus (EM) were determined according to ASTM method D (ASTM, 2002) with an Instron Testing Machine (Santam, Tehran, Iran) equipped with a tension cell of 100N. The films were cut to 60 mm 10 mm. The area of film used for each experiment was 60 mm 10 mm. However, 20 mm of the films were within the jaws, so the initial length of the film was taken as 40 mm. The thickness of the films was measured at different points with micrometer and the average was acquired. The initial cross-sectional area of film cuts were 10 mm average thickness in mm. The film cuts were conditioned at 27 C
4 Academia Journal of Food Research; Raisi-Nafchi et al. 004 Figure 1. Light absorbance of carboxymethylcellulose (CMC) and alginate (ALG) filmogenic dispersions and their blends incorporated with 8% w/w of Zataria oil (ZO). and 60 ± 5% relative humidity by placing them in desiccators over saturated solution of Mg(NO 3) 2.6H 2O for two days. The tensile strength test was then performed by stretching the film cut at speed of 50 mm/min. The software of testing machine directly provided the tensile strength, elongation at break and elastic modulus of the films. All the mechanical tests were carried out at room temperature (Bonilla et al., 2014). Solubility measurement of films The films were cut into 20 mm radius disc and then dried in a vacuum oven (Fan Azma Gostar, Tehran, Iran) at 70 C for 2 h and then weighed for the initial dry mass. Then, the dried films were immersed into 50 ml capped falcon tubes containing 25 ml of distilled water and placed inside the shaker oven (Jal Tajhiz Labtech. co. Ltd. Tehran, Iran) for 24 h at 25 C. Thereafter, the solution was filtered through Whatman filter paper (no. 1) to recover the remaining undissolved film. The remaining film pieces were placed in the vacuum oven (Fan Azma Gostar, Tehran, Iran) of 70 C for 2 h and thereafter, weighed to determine the final dry mass of film. The percentage of weight losing was taken as water solubility of the films (Gomez-Estaca et al., 2010). Water vapor permeability of films Water vapor permeability (WVP) of the film samples was examined using aluminum cups filled with 20 g silica gel to produce 0% relative humidity below the film. The film cuts were conditioned at 27 C and 60 ± 5% relative humidity by placing them in desiccators by saturated solution of Mg(NO 3) 2.6H 2O for three days. After taking the initial weight of the test cups, they were placed in a box. The weight gain of the cups was measured at 3 h intervals during per day using electronic balance (Acculab, Sartorius group, Germany). A plot of weight gain (g) against time (h) for each cup was prepared. The slope of the linear portion of this plot showed the amount of water vapor diffusion through the film per time unit and was expressed as gram unit per time unit (g/h). Water vapor transmission rates (WVTR) of the film was calculated from the slope of the linear portion of this plot per square meter (m 2 ) and expressed as g/m 2. h. The WVP was calculated using the formula: WVP (g.mm/m 2.kPa.h) = [(WVTR T)] / ΔP. T is the film thickness (mm) and ΔP is the partial water vapor pressure difference (kpa) between the two sides of
5 Academia Journal of Food Research; Raisi-Nafchi et al. 005 Table 1. Density, ph, conductivity, Zeta-potential and particle size of carboxymethylcellulose (CMC) and alginate (ALG) filmogenic dispersions and their blends incorporated with 10 % w/w of Zataria oil (ZO). Filmogenic dispersions Density (mg/ml) ph Conductivity (µs/cm) Zeta-potential (-mv) Particle size (nm) CMC 971 ± 9 b 7.07 ± 0.09 a 1050 ± 12 b 16.5 ± 2.0 b 582 ± 35 b ALG 998 ± 11 a 6.19 ± 0.09 b 76 ± 3 d 8.0 ± 0.5 d 597 ± 28 b CMC/ALG 988 ± 10 ab 6.47 ± 0.06 b 393 ± 8 c 19 ± 0.8 b 665 ± 20 a CMC/ZO 918 ± 7 e 7.17 ± 0.07 a 1150 ± 16 a 27 ± 1.5 a 435 ± 20 c ALG/ZO 958 ± 6 c 6.32 ± 0.08 b 87 ± 7 d 13 ± 1.2 c 243 ± 12 e CMC/ALG/ZO 940 ± 7 d 6.66 ± 0.08 b 435 ± 9 c 28 ± 2.0 a 370 ± 12 d The values are expressed as means ± standard deviation for at least three independent experiments. Mean values with different small letters within a column are significantly different as analyzed by Duncan test at (p < 0.05). the film ( kpa at 27 C) (Bonilla et al., 2014). Swelling test of films The film were cut into 20 mm radius disc and then dried in a vacuum oven (Fan Azma Gostar, Tehran, Iran) at 70 C for 2 h and then weighed for the initial dry mass. The film cuts were immersed into a 50 ml falcon tube containing 25 ml of the distilled water. The samples were kept at room temperature for 1 h. Each sample was taken out of the tubes, wiped between filter papers to remove the excess surface water and were weighed for final weight of swollen film. The percentage of weight gaining was taken as water swelling (WS) percentage of the films. Atomic force microscopy of the films The surface morphology of the films was analyzed using Olympus atomic force microscope instrument system (California, USA) according to manual instruction. The images were acquired in air on an anti-vibration bench and within an acoustic enclosure. Single-beam silicon cantilevers tips (PPP-NCHR-10) were used for data acquisition. Statistical analysis All the tests were performed in at least three independent experiments and expressed as the mean values ± standard deviations. The significant differences between means were analyzed by Duncan test at P<0.05 using statistical package for the social sciences (SPSS, Abaus Concepts, Berkeley, CA) software. RESULTS AND DISCUSSION Density of FD The density of ALG was higher as compared to CMC. In addition, ZO significantly reduced (p < 0.05) the density of CMC and ALG and their blends CMC/ALG (Table 1), conforming to other researches (Sanchez-Gonzalez et al., 2009, 2011). The CMC/ZO and ALG accounted for the lowest and highest densities, respectively. The decrease in the density might be attributed to the lower density of ZO rather than water, although, the rise in the intermolecular distance among FD molecules was attributed to ZO (Sanchez-Gonzalez et al., 2009, 2011). ph of FD As results showed, ph value of ALG was lower than that of CMC. ZO had no significant (p > 0.05) impact on the ph value of CMC, ALG and CMC/ALG. CMC/ZO and ALG accounted for the highest and lowest ph values, respectively (Table 1). Other literatures pointed out that when essential oil content increase, ph of different hydrogels decreases(sanchez-gonzalez et al., 2009, 2011). Adding ZO constant ph of CMC and ALG and their composites may be linked to the buffer capacity of CMC and ALG and the neutralization of ZO acidic compounds (Fu et al., 2011). Conductivity of FD According to the light of aforementioned results, ALG showed lower conductivity compared to CMC. In addition, ZO significantly (p < 0.01) increased the conductivity of all FD. The ALG and CMC/ZO accounted for the lowest and highest conductivity, respectively (Table 1). The conductivity of FD generally rests on how many electric charges (cations and anions ions) are in an electric field. Given the presence of carboxyl and hydroxyl groups, CMC and ALG had negative charges to which the high conductivity of pure CMC and ALG could be attributed. At the same time, the rise in the conductivity of FD caused by the addition of ZO could be mainly attributed to the some acidic components of ZO. Ionization of these acidic compounds increases the total negative charges of FD, hence, conductivity increased (Clements, 2007).
6 Academia Journal of Food Research; Raisi-Nafchi et al. 006 Table 2. Viscosity (mpa.s) of carboxymethylcellulose (CMC) and alginate (ALG) filmogenic dispersions and their blends incorporated with 8 % w/w of Zataria oil (ZO) at different shear rates. Filmogenic dispersions Shear rate (RPM) CMC 70 ± 4 a 84 ± 4 a 93 ± 5 a 112 ± 4 a ALG 8 ± 1 c 12 ± 1 d 21 ± 2 e 27 ± 2 e CMC/ALG 8 ± 1 c 20 ± 2 c 40 ± 3 c 56 ± 3 c CMC/ZO 77 ± 5 a 86 ± 4 a 95 ± 5 a 120 ± 5 a ALG/ZO 8 ± 1 c 12 ± 1 d 26 ± 2 d 35 ± 2 d CMC/ALG/ZO 24 ± 3 b 32 ± 3 b 51 ± 4 b 73 ± 3 b The values are expressed as means ± standard deviation for at least three independent experiments. Mean values with different small letters within a column are significantly different as analyzed by Duncan test at (p < 0.05). ζ-potential of FD The ζ-potential values (surface charge) of CMC and ALG and their composites were negatively related with the ζ- potential value of CMC higher than ALG. At the same time, ZO highly increased (p < 0.05) the ζ-potential of CMC and ALG and their composites. The lowest and highest ζ- potential values belong to ALG and CMC/ALG/ZO, respectively (Table 1). Increased ζ-potential of different hydrogels may be due to rise in the essential oil content found by other literatures (De Oliveira et al., 2014; Sanchez-Gonzalez et al., 2011). A rise in the negative charges on the surface of CMC and ALG and their composites by the addition of ZO can be attributed to the interaction among polymer molecules and ZO droplets as well. The interaction between ZO (negative charge) and CMC and ALG polymer chains (negative charges) increases the total negative charges of particles in the FD (Huang et al., 2001; Clements, 2007). Particle size of FD According to the results, CMC had lower particle size as compared to ALG. At the same time, upon mixing CMC with ALG remarkably, particle size of the composite dispersion as well as, pure CMC and ALG increased. ALG/CMC mix accounted for the highest particle size (Table 1). ZO caused a significant (p < 0.05) loss in the particle size of CMC and ALG and their composites, while the lowest particle size belongs to ALG/ZO. Any losses in particle size might be mainly attributed to the dispersive activity of ZO after interaction with polymer chain. Appropriate dispersion of ZO in the FD lowered polymer particles aggregation, decreased particle sizes (Salvia- Trujillo et al., 2013; Zhong et al., 2010). On the other side, CMC and ALG with negative charge have been proven to present interfacial activity and can interact with ZO droplets; hence, ZO can modify the electrical surface charges of polymer particles and the ζ-potential (Fu et al., 2011; Zhao et al., 2011). Adding ZO to CMC and ALG and blends caused an increase in the electrical net charge on the surface of polymer particles. The increase in the ζ- potential caused by the addition of ZO resulted in a strong electrostatic repulsion among particles whereby increasing the stability of FD. If the particles charges are sufficiently high, the solution may remain stable versus aggregation given electrostatic repulsion, so particle sizes are hereby lowered (Huang et al., 2001; Liu et al., 2012; Yang et al., 2013). Accordingly, upon adding ZO to FD, the mean particle size significantly decreased, leading to smaller particles with higher electrical negative charges. Viscosity of FD According to results, CMC had higher viscosity than ALG. At the same time, CMC/ALG showed a lower viscosity than CMC and a higher viscosity than ALG (Table 2). The viscosity of simple and composite dispersions evaluated in the present research was raised upon increasing the ZO content and also by increasing shear rates in the analyzed shear rate range. Thus, ZO incorporation led to a substantial increase in the viscosity. It should be noted that these effects were more evident at higher shear rates (Table 2). Many literatures reported an increase in the viscosity of different hydrocolloids as well as, increase in essential oil (Sanchez-Gonzalez et al., 2009, 2011). The viscosity (resistance to shear stress) of a liquid rests on the size and shape of its particles, the attraction among the particles and the interaction between water and the particles (Clements, 2007; Xiao et al., 2012). The increase in the viscosity of the FD in the presence of ZO can be due to any rise in the interaction forces between polymer chain and ZO droplets (Fu et al., 2010; Yang et al., 2013). On the other hand, final viscosity is affected by polymer particle net charges as well as particle size. By addition of ZO, the particle size decreased while the particle net charge increased. The decrease in the particle sizes increases the surface to volume ratio and the contact area between the particles thereby resulting in an increase in the viscosity of the FD (Salvia-Trujillo et al., 2013). The increase in the shear rate also caused an increase in the physical interactions among the adjacent polymer chains,
7 Academia Journal of Food Research; Raisi-Nafchi et al. 007 Table 3. Anti-oxidant power of carboxymethylcellulose (CMC) and alginate (ALG) filmogenic dispersions and their blends incorporated with 8% w/w of Zataria oil. (ZO). Filmogenic dispersions Anti-oxidant power against ABTS DPPH CMC - - ALG - - CMC/ALG - - CMC/ZO 702 ± 45 b 654 ± 34 b ALG/ZO 1100 ± 90 a 986 ± 60 a CMC/ALG/ZO 615 ± 30 c 565 ± 25 c Anti-oxidant power of samples was calculated by using the following formula: [1000/IC50] 100. The values are expressed as means ± standard deviation for at least three independent experiments. Mean values with different letters within a column are significantly different as analyzed by Duncan test at (p < 0.05). Table 4. Tensile strength (MPa), elastic modulus (MPa) and elongation at break (%) of carboxymethylcellulose (CMC) and alginate (ALG) films and their composites incorporated with 8% w/w of Zataria oil (ZO). Films Tensile strength (MPa) Elastic modulus (MPa) Elongation at break (%) CMC 37 ± 1.5 a 540 ± 15 a 12 ± 1.5 e ALG 21 ± 1.4 c 170 ± 7 d 17 ± 1.2 d CMC/ALG 21 ± 1.2 c 453 ± 12 b 33 ± 1.7 b CMC/ZO 25 ± 1.0 b 448 ± 10 b 17 ± 2.0 d ALG/ZO 16 ± 1.0 d 138 ± 5 e 23 ± 2.2 c CMC/ALG/ZO 14 ± 0.8 e 380 ± 8 c 48 ± 2.7 a The values are expressed as means ± standard deviation for at least three independent experiments. Mean values with different letters within a column are significantly different as analyzed by Duncan test at (p < 0.05). hence, it significantly increased the viscosity in the range of the tested shear rate (Zhong et al., 2010). Antioxidant activity of FD Antioxidant activities of the FD and their composites versus ABTS, DPPH radicals were further assessed (Table 3). Pure ALG and CMC had a slight antioxidant activity (Tomida et al., 2012). CMC and ALG and their composites which were combined with ZO had potent anti-oxidant activity. Many previous literatures reported similar DPPH and ABTS scavenging capacities for ZO (Kavoosi and Rabiee, 2015; Kavoosi et al., 2012). DPPH and ABTS radical scavenging capacity of ZO can be a great measure of hydrogen atom and/or the electron donating capacity of ZO. Once ZO is considered (as an anti-oxidant), a hydrogen atom or an electron is transferred to DPPH and ABTS radicals, consequently convert them to a non-radical state (Floegel et al., 2011).Thus, CMC and ALG and their blends which were incorporated with ZO, had potent antioxidant capacity. It has been reported that oxidative corrosion may play crucial role in the reduction of the nutritional and sensory quality of food products (Gomez-Estaca et al., 2014). Oxidation leads to a significant loss of nutritional worth of food products by damaging vitamins and unsaturated fatty acids. Oxidation also affects sensory quality of food products including color, texture and taste and shortens the shelf-life of food (Tongnuanchan and Benjakul, 2014). The antioxidant activity of CMC/ZO and ALG/ZO imply that such products can effectively reduce the oxidative deterioration of food stuff. Mechanical properties of films Table 4 presents results of mechanical properties of CMC, ALG and CMCA/ALG films. Tensile strength (TS) and elastic modulus (EM) of pure CMC films were higher as compared to that of ALG films. CMC/ALG composite film had lower TS and EM than CMC. ALG film showed higher elongation at breaks than CMC films. CMC/ALG composite films had higher elongation at break than pure CMC and ALG. The results showed low compatibility of ALG with CMC for producing a composite film with high tensile but with strong compatibility of them to produce a flexible composite film (Sirvio et al., 2014). ZO lowered tensile strength and EM of CMC and ALG films and their composites, while increasing elongation at break of them (Table 4). The results demonstrated that the tensile strength and EM of the films and their composites decreased by adding ZO which is in agreement with the results of Sanchez-Gonzalez et al. (2009), Liakos et al.
8 Academia Journal of Food Research; Raisi-Nafchi et al. 008 Table 5. Solubility, water vapor permeability (WVP) and swelling of carboxymethylcellulose (CMC) and alginate (ALG) films and their composites incorporated with Zataria oil (ZO). Films Solubility (%) WVP (mg.mm/m 2.h) Swelling (%) CMC 63 ± 4 c 740 ± 25 c 700 ± 20 a ALG 85 ± 7 ab 753 ± 20 c 240 ± 9 e CMC/ALG 43 ± 4 d 744 ± 30 c 488 ± 11 c CMC/ZO 75 ± 7 b 880 ± 37 b 616 ± 14 b ALG/ZO 89 ± 8 a 915 ± 23 b 205 ± 8 f CMC/ALG /ZO 55 ± 5 c 1037 ± 45 a 408 ± 8 d The values are expressed as means ± standard deviation for at least three independent experiments. Mean values with different small letters within a row are significantly different as analyzed by Duncan test at (p < 0.05). (2014), Benavides et al. (2012) and Rojas-Grau et al. (2007). Reduction of films tensile strength in the presence of ZO is probably mainly attributed to the formation of inter-molecular interaction between hydroxyl/carboxyl groups of CMC and ALG and hydroxyl groups of ZO components (Liakos et al., 2014). Hence, the original bonds/interactions between polymer chains could be replaced with new bonds/interactions between polymer molecules and ZO. These events amend polymer matrix integrity and reduce tensile strength of the films (Goh et al., 2012). EM is a measure of the stiffness (hardness) of the film. A stiff material has high EM and changes its shape only slightly under elastic loads. Reduction in the film rigidity in the presence of ZO could be mainly attributed to replacement of original bonds between polymer chains with new bonds between polymer chain and ZO droplets which caused an increase in the segmental mobility of polymer chains (Sanchez-Gonzalez et al., 2009; Pastor et al., 2013). In the presence of ZO, the flexibility of the films increased, which was in accordance with the results of Maizura et al. (2007) on the lemongrass oil incorporated to alginate films and Benavides et al. (2012) on the alginate film incorporated with oregano oil. Elongation at break is an indication of flexibility and extensibility of the films. Increasing the flexibility of the films in the presence of ZO could be mainly attributed to replacement of original bonds between polymer chains with new bonds between CMC and ALG (Liakos et al., 2014). By this effect, the segmental mobility of polymer chains increases which leads to more sliding effect of polymer chains versus each other, thus, flexibility of films increased (Sanchez-Gonzalez et al., 2011). lower than CMC films. All CMC, ALG and CMC/ALG had similar WVP values. The results established the strong compatibility of CMC with ALG concerning the production of a composite film with a low solubility and swelling (Benavides et al., 2012; Rojas-Grau et al., 2007). ZO was led to a significant (p < 0.05) rise in water solubility and WVP and a significant (p < 0.05) decrease in the swelling of the films. This increase in the water solubility might be caused by establishing of CMC-ZO and ALG-ZO interactions, which weakens the interactions stabilizing the polymer network (Benavides et al., 2012; Rojas-Grau et al., 2007). ZO can interact with hydroxyl groups of CMC and ALG chain and competitively weaken polymer chain-to-chain Hydrogen Bridge. This effect reduces CMC and ALG matrix network integrity and consequently, causes an increase in the solubility of the films (Goh et al., 2012). At the same time, the original hydrogen binding between CMC and ALG chains replaced with the new hydrogen bonds between hydroxyl groups of polymer and ZO. This event increases the distance between polymer chain and introduced twisting pores in the polymer matrix; thus, water vapor transmission across the film samples increased (Liakos et al., 2014). Due to hydroxyl and/or carboxyl groups, CMC and ALG are hydrophilic materials so that they can absorb huge amount of water molecules (Sanchez-Gonzalez et al., 2011). ZO could reduce swelling capacity of the films which might be mainly attributed to hydrophobic nature of the ZO. Hydroxyl groups of CMC and/or ALG can interact with ZO components through hydrogen binding and whereby the interaction between polymer chain and ZO was increased. This event saturates CMC and ALG network with ZO; hence, water molecules cannot interact with CMC and ALG whereby swelling decreases (Pastor et al., 2013). Water binding capacity of film Table 5 presents results of water binding capacity such as water solubility, WVP and swelling. CMC film showed lower solubility as well as, higher swelling compared to ALG film. CMC/ALG composite films were shown to have lower solubility than pure CMC and ALG films. CMC/ALG composite films had higher swelling than pure ALG and Atomic force microscopy Figure 2 illustrates atomic force microscope images of CMC and ALG films and CMC/ALG composite films. Incorporation of ZO induced the changes in the surface topography of the simple and composite films. Upon addition of ZO the surface roughness was increased. This means that ZO decreased CMC and ALG chain association
9 Academia Journal of Food Research; Raisi-Nafchi et al. 009 Figure 2. Atomic force microscope micrographs of the surface of the carboxymethylcellulose (CMC), alginate (ALG) and CMC/ALG films incorporated with Zataria oil (ZO). in the filmogenic dispersion and during the film drying and casting (Liakos et al., 2014; Pastor et al., 2013). Accordingly, ZO had an impact on the surface morphology and structure of pectin film. The change in the film morphology will affect the mechanical and water binding properties of films. Conclusion The last but not the least, CMC, on the other hand, showed the highest ph, conductivity, ζ-potential and viscosity. In addition, ALG was accounted for highest density, particle size, light barrier and antioxidant values. ZO lowered the density and particle size of CMC and ALG FD and their composites. It also caused a significant rise in the ζ- potential, viscosity, light barrier and antioxidant properties of CMC and ALG as well as, their composites. Accordingly, when ZO was added, oil percentage, polymer type and polymer blending affected density, ph, ζ- potential, average particle sizes, size distribution, viscosity and light barrier of CMC and ALG and their composites were affected by them. Changes in the physical properties of CMC and ALG implied an interaction between the molecules of CMC and ALG and ZO components. Such interactions might influence mechanical properties of the films casted from the FD. CMC film accounted for the highest tensile strength while ALG film showed the highest flexibility. A significant decrease in tensile strength and increase in elongation at break of CMC and ALG films and their composites resulted from ZO. The improved antioxidant activities denoted on potential of CMC and ALG in such applications as food preservation. Above all, much more in vivo researches are required to shed lights on biocompatibility of such materials. It is accordingly promising that forthcoming researches focus on the applications of CMC and ALG (enriched with essential oil) to in vivo systems to evaluate their biocompatibility.
10 Academia Journal of Food Research; Raisi-Nafchi et al. 010 ACKNOWLEDGEMENTS This work was supported by the financial support from Shiraz University (grant No. 88-GRAGRST-108). REFERENCES ASTM (2002). Standard test method for tensile properties of thin plastic sheeting: D annual book of American society for testing materials, West Conshohocken, PA, USA. Benavides S, Villalobos-Carvajal, R, Reyes JE (2012). Physical, mechanical and antibacterial properties of alginate film: Effect of the crosslinking degree and oregano essential oil concentration. J. Food Eng. 110: Bonilla I, Fortunati E, Atares L, Chiralt A, Kenny JM (2014). Physical, structural and antimicrobial properties of poly vinyl alcohol chitosan biodegradable film. Food Hydrocoll. 35: Clements DJ (2007). Critical review of techniques and methodologies for characterization of emulsion stability. Crit. Rev. Food Sci. Nutr. 47: De Oliveira EF, Paula HC, DE Paula RC (2014). Alginate/cashew gum nanoparticles for essential oil encapsulation. Colloid. Surface B. 113: Floegel A, Kim DO, Chung SJ, Koo SI, Chun OK (2011). Comparison of ABTS/DPPH assays to measure antioxidant capacity in popular antioxidant-rich US foods. J. Food Compos. Anal. 24: Fu S, Thacker A, Sperger DM, Boni RL, Buckner IS, Velankar S, Block LH (2011). Relevance of rheological properties of sodium alginate in solution to calcium alginate gel properties. AAPS Pharm. Sci. Tech. 12: Goh CH, Heng PWS, Chan LW (2012). Cross-linker and non-gelling Na + effects on multi-functional alginate dressings. Carbohyd. Polym. 87: Gomez-Estaca J, Lopez-Dedicastillo C, Hernandez-Munoz P, Catala R, Gavara R (2014). Advances in antioxidant active food packaging. Trend. Food Sci. Tech. 35: Huang X, Kakuda Y, Cui W (2001). Hydrocolloids in emulsions: particle size distribution and interfacial activity. Food Hydrocoll. 15: Kavoosi G, Rabiei F (2015). Z. Multiflora: Chemical and Biological Diversity in the Essential Oil. J. Essent. Oil. Res. 27: Kavoosi G, Rahmatollahi A, Dadfar SM, Mohammadi PA (2014). Effects of essential oil on the water binding capacity, physico-mechanical properties, antioxidant and antibacterial activity of gelatin films. LWT- Food Sci. Technol. 57: Kavoosi G, Teixeira da Silva JA, Saharkhiz MJ (2012). Inhibitory effects of Z. multiflora essential oil and its main components on nitric oxide and hydrogen peroxide production in lipopolysaccharide-stimulated macrophages. J. Pharm. Pharmacol. 64: Lee KY, Mooney DJ (2012). Alginate: properties and biomedical applications. Prog. Polym. Sci. 37: Liakos I, Rizzello L, Scurr DJ, Pompa PP, Bayer IS Athanassiou A (2014). All-natural composite wound dressing films of essential oils encapsulated in sodium alginate with antimicrobial properties. Int. J. Pharm. 463: Liu Q, Han JC, Zhang YG, Li SM Li J (2012). Antimicrobial and antioxidant activities of carboxymethyl cellulose edible films incorporated with rosemary extracts on fresh beef during refrigerated storage. Adv. Mat. Res. 554: Maizura M, Fazilah A, Norziah MH, Karim AA (2007). Antibacterial activity and mechanical properties of partially hydrolyzed sago starchalginate edible film containing lemongrass oil. J. Food Sci. 72: Pastor C, Sanchez-Gonzalez L, Chiralt A, Chafer M, Gonzalez-Martinez C (2013). Physical and antioxidant properties of chitosan and methylcellulose based films containing resveratrol. Food Hydrocoll. 30: Pawar SN, Edgar KJ (2012). Alginate derivatization: A review of chemistry, properties and applications. Biomaterials. 33: Ramirez C, Gallegos I, Ihl M, Bifani V (2012). Study of contact angle, wettability and water vapor permeability in carboxymethylcellulose based film with murta leaves (Ugni molinae Turcz) extract. J. Food Eng. 109: Rojas-Grau MA, Avena-Bustillos RJ, Olsen C, Friedman M, Henika PR, Martin-Belloso O, Pan Z, Mc Hugh TH (2007). Effects of plant essential oils and oil compounds on mechanical, barrier and antimicrobial properties of alginate-apple puree edible films. J. Food Eng. 81: Sajed H, Sahebkar A, Iranshahi M (2013). Z. multiflora Boiss. (Shirazi thyme)-an ancient condiment with modern pharmaceutical uses. J. Ethnopharmacol. 145: Salvia-Trujillo L, Rojas-Graü MA, Soliva-Fortuny R, MArtín-Belloso O (2013). Effect of processing parameters on physicochemical characteristics of microfluidized lemongrass essential oil-alginate nanoemulsions. Food Hydrocoll. 30: Sanchez-Gonzalez L, Chiralt A, Gonzalez-Martinez C, Chafer M (2011). Effect of essential oils on properties of film forming emulsions and films based on hydroxypropylmethylcellulose and chitosan. J. Food Eng. 105: Sanchez-Gonzalez L, Vargas M, Gonzalez-Martinez C, Chiralt A, Chafer M (2009). Characterization of edible films based on hydroxypropylmethylcellulose and tea tree essential oil. Food Hydrocoll. 23: Shah N, Ul-Islam M, Khattak WA, Park JK (2013). Overview of bacterial cellulose composites: A multipurpose advanced material. Carbohyd. Polym. 98: Shi Z, Zhang Y, Phillips GO, Yang G (2013). Utilization of bacterial cellulose in food. Food Hydrocoll. 35: Sirvio JA, Kolehmainen A, Liimatainen H, Niinimaki J, Hormi OEO (2014). Biocomposite cellulose-alginate films: Promising packaging materials. Food Chem. 151: Tomida H, Yasufuku T, Fujii T, Kondo Y, Kai T, Anraku M (2010). Polysaccharides as potential antioxidative compounds for extendedrelease matrix tablets. Carbohyd. Res. 345: Tongnuanchan P, Benjakul S (2014). Essential Oils: Extraction, Bioactivities, and Their Uses for Food Preservation. J. Food Sci. 79: R Xiao Q, Tong Q, Lim LT (2012). Pullulan-sodium alginate based edible films: Rheological properties of film forming solutions. Carbohyd. Polym. 87: Yang Y, Campanella OH, Hamaker BR, Zhang G, Gu Z (2013). Rheological investigation of alginate chain interactions induced by concentrating calcium cations. Food Hydrocoll. 30: Zhao GH, Kapur N, Carlin B, Selinger E, Guthrie JT (2011). Characterisation of the interactive properties of microcrystalline cellulose-carboxymethyl cellulose hydrogels. Int. J. Pharm. 415: Zhong D, Huang X, Yang H, Cheng R (2010). New insights into viscosity abnormality of sodium alginate aqueous solution. Carbohyd. Polym. 81: Cite this article as: Raisi-Nafchi M, Kavoosi G, Nasiri SM (2016). Physico-mechanical and antioxidant properties of carboxymethylcellulose and alginate dispersions and essential oil based films for use as food packaging materials. Acad. J. Food. Res. 4(1): Submit your manuscript at: